SATURATED HYDROCARBON POLYMERIC BINDER FOR SATURATED HYDROCARBON POLYMERIC BINDER FOR ADVANCED SOLID...
Embed Size (px)
Transcript of SATURATED HYDROCARBON POLYMERIC BINDER FOR SATURATED HYDROCARBON POLYMERIC BINDER FOR ADVANCED SOLID...
SATURATED HYDROCARBON POLYMERIC BINDER FOR
ADVANCED SOLID PROPELLANT AND HYBRID SOLID GRAIN
PERIOD COVERED: August 1, 1967 - December 31, 1967
This work was performed for the Jet Propulsion Laboratory, California Institute of Technology, as sponsored by the National Aeronautics and Space Administration under Contract NAS 7-100.
Report Edited By: James E. Potts
ucc Contributors: A. C. Ashcraft, Jr. J. E. Potts E. M. Sullivan E. W. Wise
Publication Date: January 19, 1968
Jet Propulsion Laboratory Contract No. 951210
Technically Managed By: H. E. Marsh, Jr. - JPL
UNION CARBIDE CORPORATION CHEMICALS AND PLASTICS
Polymer Research and Development Bound Brook, New Jersey
TECHNICAL CONTENT STATEMENT
This report contains information prepared by Union Carbide Corporation, Chemicals and Plastics Operations Divi- sion, under J.P.L. subcontract. Its content is not necessarily endorsed by the Jet Propulsion Laboratory, California Institute of Technology or the National Aeronautics and Space Admini- stration.
I1 . 111.
IV . V.
TABLE OF CONTENTS
Page No. - 1
SCOPE OF PROJECT.............................
A. Telomer Preparation and Evaluation....... 3 B. Telomer Preparation - Composite Batches
I and II................................. 6 C. Telomer Preparation in the Continuous
Stirred Autoclave Reactor...... . . ..... ... 12 D. Telomer Reactions - Dehydrobromination
and Ozonolysis ........................... 18 1. Studies on 24-EMS-122................ 19 2. Studies on 25-EMS-22................. 21 3. Studies on Composite Batch I......... 2 4 4. Summary of Reaction.Studies. ......... 28
VI . VI1 .
PLANS FOR FUTURE WORK....... ................. 29
Union Carbide Corporation, Chemicals and Plastics Operations Division has agreed to assist the Jet Propulsion Laboratory, California Institute of Technology, on a level of effort basis, in the development of a new or improved polymeric binder for advanced solid propellant and hybrid propellant grains. The general objectives are described in Quarterly Report No. 1. This report makes the transition from the exploratory polymer research phase of the work to the product definition or development phase.
Additional samples of ethylene/neohexene telomers have been prepared by a batch process in the stirred auto- clave reactor using bromoacid and bromoester telogens. From our exploratory telomerization studies we have found that the bromoacid CTAC and the bromoester CTAD are the most use- ful telogens. With thernwe have achieved the best control of functionality at useful molecular weights.
The product definition and development phase of the work has begun with the start up of operations on the continuous stirred autoclave reactor. Reaction conditions and product goals established in the exploratory research phase are serving as points of reference for telomer synthe- sis in the continuous reactor.
A total of six runs have been made in the continuous reactor using the bromoacid telogen CTAC. Telogen concen- tration and reactor residence times were varied and found to give useful and predictable control over the molecular weight without substantially affecting the functionality. Uniform products of high functionality were obtained in these start- up runs.
Conditions for efficiently conducting the dehydro- bromination/oxidation reaction sequence have been established using samples prepared in the batch reactor with both CTAC and CTAD telogens. Nearly quantitative conversion of bromide fun- ctionality to carboxyl functionality has been achieved along with no loss of the original carboxylic functional groups.
- 1 -
111. SCOPE OF PROJECT
The scope of this work has not changed from the program outlined in the work statement.
In our previous report we introduced several new halogen containing telogens, or chain transfer agents, and discussed telomers of ethylene and neohexene prepared with the aid of these new telogens. The terminal functional groups on the telomers were derived from the particular telogen used. which were either w-bromoacids or w-bromoesters. Three methods were discussed for converting the terminal bromide into a useful carboxylic acid group. be effective: dehydrobromination of the w-bromide to give a terminal double bond, followed by ozonolysis with oxi- dative workup to give a carboxyl group. The other methods (displacement by cyanide followed by hydrolysis, or coupling via S I ) were found to'be effective in model compounds, but failed when applied to the o-bromo acid telomers.
The most promising telogens gave telomers
Only one was found to
In this repoFt we will present the results of telomer syntheses using a new telogen, two series of batch telomerizations using our most effective telogens, and we will compare these results with those we obtained when a continuous stirred autoclave reactor was used for the telo- merizations instead of a batch reactor.
The dehydrobromination/ozonolysis route to carboxyl end groups was further perfected during this period and used to convert our w-bromo acid and ester telomers to carboxyl terminated products. in the Technical Discussion to follow.
These results will be reported in detail
- 2 -
V. TECHNICAL DISCUSSION
A. Telomer Preparation and Evaluation
The bromoester telogen "CTAF" was evaluated in telo- merizations number 24-EMS-132, 133, 135 and 25-EMS-6. The production data for these runs is summarized in Table I. Run 135 is a repeat of 133, made necessary because a purging opera- tion, which occurred during the preparation for-run 133, caused a loss of some of the neohexene charged to the reactor. For this reason the product from run 133 had a higher ethylene con- tent than planned. This product is a grease, showing evidence of polyethylene crystallinity.
Reaction time and telogen/monomer molar ratio were varied in these runs. The average level of initiator (AIBN) was maintained at the same value through all the runs. effect of reaction time is shown by the increasing yields: 19, 41 and 90 grams for 3.42, 6.25 and 12.25 hours respectively.
Table I1 summarizes the results obtained upon analy- sis of these products. As expected, the molecular weights are higher for the runs at lower telogen/monomer ratios, however, the functionalities are rather low.
The nitrogen contents (from AIBN) show that a sub- stantial amount of initiation of polymer chains, -25%, is accomplished by the initiator itself rather than being largely due to the radical derived from the telogen by chain transfer. This, together with the molecular weights obtained, show that CTAF is a sluggish chain transfer agent compared to CTAC and CTAD. Use of a higher concentration of CTAF and a lower con- centration of initiator could alleviate this problem.
The lower bromine content of run 135 is due to de- hydrobromination occurring during recovery of the telomer. The infrared spectrum of this product shows a strong c = c* absorbtion at 10.35~~ corresponding to a trans-internal double bond. ducts. In addition to this, a second carbonyl band at 5 . 8 6 ~ is observed (main band at 5.751-1). Since COOH is absent, this is most consistent with the presence of a,B-unsaturated ester end groups in this telomer. These could only be derived from an a-bromoester end group resulting from initiation by an a- bromoester radical, presumably formed by hydrogen atom abstrac- tion rather than bromine atom abstraction from CTAF. This
This is not present in the spectra of the other pro-
- 3 -
RUN # 24-EMS
Telogen Telogen, gms. Solvent, 1:l Benzene:Butanol/,gms. Initiator Initiator, gms. Neohexene, gms . Ethylene, gms . FED DURING REACTION
Telogen, gms. Solvent; gms. Initiator, gms.
Temperature, C Pressure, mpsi
Time, hrs .
Yield, gms. Conversion, % Conversion Rate, %
14.2 129 . 8
6.00 15.00 3.42
.13 679.6 257
3.25 8.00 6.25
.13 679.6 254
14.2 128.0 1.17
9.00 14.30 6.25
2 5 -EMS - 6
.26 679.6 254
14.2 128.5 2.34
10 . 50 17.25 12.25
- 4 -
RUN # 24-EMS-
Brookfield Visc., Cps Specific Visc., @ 8OoC Description
Molecular Wt. (benzene)
Oxygen, Wt. % Chlorine, Wt.